### Delft University of Technology

### Effects of Defect and Temperature on the Mechanical Performance of WS2

### A Multiscale Analysis

Tang, Hongyu; Hu, Dong; Cui, Zhen; Ye, Huaiyu; Zhang, Guoqi DOI

10.1021/acs.jpcc.0c09897 Publication date

2021

Document Version Final published version Published in

Journal of Physical Chemistry C

Citation (APA)

Tang, H., Hu, D., Cui, Z., Ye, H., & Zhang, G. (2021). Effects of Defect and Temperature on the Mechanical Performance of WS2: A Multiscale Analysis. Journal of Physical Chemistry C, 125(4), 2680-2690.

https://doi.org/10.1021/acs.jpcc.0c09897 Important note

To cite this publication, please use the final published version (if applicable). Please check the document version above.

Copyright

Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy

Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.

This work is downloaded from Delft University of Technology.

### of WS

_{2}

### : A Multiscale Analysis

### Hongyu Tang,

∥### Dong Hu,

∥### Zhen Cui, Huaiyu Ye, and Guoqi Zhang

### *

Cite This:J. Phys. Chem. C 2021, 125, 2680−2690 Read Online

### ACCESS

Metrics & More Article Recommendations### *

sı Supporting InformationABSTRACT: This paper analyzes the mechanical properties of

tungsten disulﬁde (WS2) by means of multiscale simulation, including

density functional theory (DFT), molecular dynamic (MD) analysis, andﬁnite element analysis (FEA). We ﬁrst conducted MD analysis to calculate the mechanical properties (i.e., Young’s modulus and critical stress) of WS2. The inﬂuence of diﬀerent defect types (i.e., point defects

and line defects) on the mechanical properties are discussed. The results
reveal that WS_{2} has a high Young’s modulus and high critical stress.
Next, the eﬀects of defect density and temperature on the mechanical
properties of the material were analyzed. The results show that a lower
defect density results in improved performance and a higher
temperature results in better ductility, which indicate that WS_{2} can
potentially be a strain sensor. Based on this result, FEA was employed to
analyze the WS_{2}stress sensor and then fabricate and analyze the device

for benchmarking. It is found that the FEA model proposed in this work can be used for further optimization of the device.
According to the DFT results, a narrower band gap WS_{2}is found with the existence of defects and the applied strain. The proposed
multiscale simulation method can eﬀectively analyze the mechanical properties of WS2 and optimize the design. Moreover, this

method can be extended to other 2D/nanomaterials, providing a reference for a rapid and eﬀective systematic design from the nanoscale to macroscale.

1. INTRODUCTION

After graphene was discovered in 2004, various
two-dimen-sional (2D) materials beyond graphene, such as
transition-metal dichalcogenides (TMDCs), MXenes, and transition-metal oxides,
have attracted extensive attention worldwide.1 Tungsten
sulﬁde (WS_{2}), as a semiconductor of TMDCs, consists of
three atomic layers of W layers sandwiched between two S
layers, which enable its Young’s modulus to be 236 ± 65 GPa
that is comparable to that of steel.2It has an indirect band gap
of∼1.9 eV and unique chemical properties, which indicate that
WS2has great potential to be applied in photonics, gas sensors,

and transistors.3−7 Beneﬁt from high Young’s modulus, WS_{2}
has been widely used forﬂexible devices, such as E-skin and
wearable sensors.8 Recently, the 2D elastic moduli and
Poisson’s ratios derived from ﬁrst-principles density functional
theory (DFT) calculations are 137 N/m and 0.22 for WS2,

respectively.9Zhang et al.10investigated the strain relaxation of
monolayer WS_{2} triangular crystals deposited on a
polydime-thylsiloxane substrate. They found that the optical spectra of
monolayer WS2depended on the range and direction of tensile

strain. Guo et al.11used WS2in a humidity sensor forﬂexible

electronic skin. Qi et al.12deposited WS2onto a polyethylene

terephthalate (PET) substrate and obtained a high-sensitive, ﬂexible, and transparent sensor with a gauge factor (GF) of 14.

However, few people considered the inﬂuence of defects on the electrical, optical, and mechanical properties of WS2.

Diﬀerent from the simple monovacancy in graphene, WS2

has more complicated defects because of its sandwiched structure.13 It is known that the WS2 monolayer exhibits

naturally formed vacancies, such as S vacancy (V_{S}) and W
vacancy (V_{W}), which have signiﬁcant impacts on the electrical
and optical properties. Through DFT analysis, Zhao et al.14
demonstrated that intrinsic three tungsten vacancies (V3W), six

sulfur vacancies (V6S), and 1W + 2S vacancies (V1W+2S) could

induce a total spin magnetic moment. Schuler et al.15analyzed the eﬀects of four diﬀerent substitutional defects on the charge localization and optical properties of WS2 through

exper-imental and theoretical analyses. Except for pristine defects, the
defects induced by external tensile strain will signiﬁcantly aﬀect
the performance of WS_{2}. Wang et al.16predicted the inﬂuence
of crack edge chirality and tip conﬁguration on the fracture
Received: November 2, 2020

Revised: January 8, 2021 Published: January 20, 2021

© 2021 The Authors. Published by

Downloaded via TU DELFT on February 9, 2021 at 07:31:49 (UTC).

toughness and crack propagation path of monolayer MoS_{2}.
However, few researchers focus on the defects’ inﬂuence on
the mechanical properties of WS_{2}, which hinders its
applications in strain sensors.

Multiscale simulations for 2D materials have been studied in diﬀerent length scales, including atomic, molecular, and device-level modeling.17,18 Mashhadzadeh et al.19−22 analyzed the mechanical properties of various nanomaterials based on molecular dynamics (MD) simulations. They also used a multiscaleﬁnite element model to study the tensile modulus of graphene-reinforced polypropylene nanocomposites and com-pare the results with experimental tensile tests. Kumar et al.23 demonstrated that interlayer interactions of three diﬀerent bilayer structures can cause band gap change by using a multiscale computational method. The elastic deformations for general bilayer structures have been established and validated via comparing the deformations with MD simulations as well as with experiments for graphene/hBN bilayer heterostruc-tures. The electrical, optical, and gas sensing properties of 2D materials have been analyzed through ﬁrst-principles anal-ysis.24,25 However, it is a lack of multiscale approach to systematically analyze the mechanical properties of WS2 with

defects.

In this study, weﬁrst perform systematic MD simulations to
investigate the mechanical properties of WS_{2}without and with
defects under tensile strain in armchair (AC) and zigzag (ZZ)
directions. The defected WS_{2}involves the fracture of WS_{2}with
initial AC and ZZ cracks and 5−8−5 defects. The mechanical
behaviors of WS_{2}are studied across diﬀerent defect densities
and diﬀerent temperatures. Moreover, we predict the potential
applications of WS_{2}in the strain sensor throughﬁnite element
analysis (FEA) and experiments. Finally, ﬁrst-principles
analysis is employed to study the inﬂuence of engineering
strain on the band structure of WS2.

2. MULTISCALE COMPUTATIONAL METHODS 2.1. First-Principles Analysis Method. Allﬁrst-principles calculations were carried out within the DFT method by Materials Studio software.26The generalized gradient approx-imation with the Perdew−Burke−Ernzerhof functional was employed. A double-sized numerical basis set plus polarized p-functional was used for our calculations. To describe the van der Waals interactions, the DFT-D (D stands for dispersion) method with TS correction was adopted.27The kinetic energy cutoﬀ of the plane wave was set to 500 eV on a Monkhorst− Pack special k-point scheme of 7 × 7 × 1 for geometry optimization and 12 × 12 × 1 k-points for band structure calculations. The maximum force and maximum displacement were set to be 0.002 Ha Å−1and 1.0 × 10−5Å, respectively. The convergence criterion for the force between atoms was 0.03 eV Å−1. Periodic boundary conditions were applied in the x and y directions. A 2× 2 × 1 supercell with an adequate 20 Å vacuum region was introduced to prevent the interactions between the adjacent layers (Figure 1).

2.2. MD Model and Methods. To investigate the
deformation and fracture properties of WS_{2}, MD simulations
were carried out using the Large-scale Atomic/Molecular
Massively Parallel Simulator (LAMMPS) package.28 Periodic
boundary conditions are applied in all three dimensions. A
monolayer WS_{2} model was placed at the center of the
simulation box as a square domain with side lengths of 75−150
Å, containing 1773 to 7452 atoms. The AC and ZZ edges are
oriented along the x and y directions, respectively. Besides, a

60 Å vacuum space is added upon the monolayer of WS2. The

monolayer WS_{2}consist of pairwise (W−S, W−W, and S−S)
and angle-bending (S−W−S and W−S−W) interatomic
interactions. Atomic interactions through WS_{2}were described
by the Stillinger−Weber (SW) potential.29,30Zhang et al.31did
a theoretical prediction of superhigh-performance
thermo-electric materials based on MoS2/WS2 hybrid nanoribbons

combined with ﬁrst-principles calculations and MD simula-tions. They veriﬁed the feasibility of SW potential in MD through DFT calculations. The ﬁtted SW parameters for monolayer WS2are listed in Tables S1 and S2. The velocities

of atoms were randomly assigned with the Gaussian distribution at the target tension temperature. Newton’s equation of motion was integrated with the Verlet algorithm. To stabilize the structure, the energy of the system was minimized by using the conjugate gradient algorithm. There-fore, after energy minimization, the models wereﬁrst relaxed at a target temperature (200−600 K) in the isothermal−isobaric ensemble with a Nose−Hoover thermostat for 50 ps, to reach their equilibrium state. The external pressure on the simulation box was removed to avoid the inﬂuence caused by the pressure variation. Then, the tension simulation at the target temper-ature was also implemented in the isothermal−isobaric ensemble. Deformation was achieved by changing the shape of the simulation box in the tension direction with a constant strain rate of 0.001 ps−1. The tension simulation stops until the engineering strain reaches 0.3. The velocity Verlet scheme with a time step of 1 fs was utilized for time integration. The average stress for the entire system was calculated by using the formula introduced by Surblys et al.32to get the stress−strain curves of the tension simulation

Ä
Ç
ÅÅÅÅÅ
ÅÅÅÅÅ
Å
É
Ö
ÑÑÑÑÑ
ÑÑÑÑÑ
Ñ
*V* *r F* *r F* *mv v*
1 1
2 ( )
*ab*
*i* *n*
*N*
*i*
*a b*
1
1 1*a* *b* 2 2*a* *b*
p

### ∑ ∑

### ∑

*σ = −*+ + = (1)

where a and b take on values x, y, z to generate the diﬀerent stress vectors. Theﬁrst term represents the viral contribution caused by intra- and intermolecular interactions. Np is the

neighbor of atom i; r_{1}and r_{2} represent the positions of the
atoms in the pairwise interaction; and F1and F2are the forces

on the atoms resulting from the pairwise interaction. The second term is the kinetic energy contribution to the total stress, where m is the mass and v is the velocity. Besides, V is the total volume of the system. In terms of uniaxial tension simulation, only the component vector on the loading direction was extracted as the stress at a speciﬁc strain. The atomic conﬁgurations were visualized by Open Visualization Tool (OVITO).33

Figure 1.Schematic of the (a) top view and side view of defect-free WS2. W atoms are shown in blue, whereas S atoms are shown in yellow.

For studying the eﬀects of natural defects in WS2, two kinds

of point defect, an S vacancy and a 5−8−5 defect, are presented in the center of WS2, as shown inFigure 2a,b. The

5−8−5 defect is a kind of point defect associated with a
“pentagon−octagon−pentagon” conﬁguration of W and S
atoms. For studying the crack edge chirality and the crack tip
structure, two kinds of line cracks, ZZ cracks and AC cracks,
are modeled and analyzed. Because of the asymmetry of the
lattice structure of WS_{2}, the ZZ crack is composed of pairs of S
atoms at its outermost atomic layer, whereas the other surface
is composed of W atoms (seeFigure 2c). The surfaces of AC
cracks are symmetric and have two diﬀerent tip structures: a
pair of S atoms (AC-S) or one W atom (AC-W) at their tips
(see Figure 2d,e). The build-up models contain 3360−3456
atoms.

2.3. Finite Element Methods. The mechanical
perform-ance of the WS_{2}-basedﬂexible device was analyzed by the ﬁnite
element model (ANSYS workbench 14.0). The model
geometry is shown in Figure 3, which consists of a ﬂexible
substrate and electrodes. Because the thickness of the WS_{2}thin
ﬁlm is much thinner than that of the substrate and electrodes,
and WS2is fully covered by the electrodes, the deformation of

WS2synchronizes with that of the substrate. In this model, we

did not consider WS_{2}to reduce the number of mesh facets and
speed up calculations. The material properties in the WS2

-basedﬂexible device are listed inTable 1. The temperature is set at 25 °C. The boundary condition is assumed that the surface of the substrate has no defects or scratches. The left

end isﬁxed, and the right end is applied with a tensile force F in the x-direction (Figure 4).

3. RESULTS AND DISCUSSION

3.1. Eﬀects of Defects on the Mechanical Perform-ance of WS2. At ﬁrst, the uniaxial tensile analysis was

performed on a stand-alone and defect-contained WS2at 300

K using the strain rate of 0.001 ps−1. The defects were divided
as point defects (2S vacancies and 5−8−5 defect) and line
defects (ZZ, AC-S, and AC-W defects). The corresponding
stress−strain curves are plotted inFigure 4. Byﬁtting the initial
stress−strain curves based on linear regression up to 1% strain,
we obtained the corresponding Young’s modulus E_{x}= 113.61
GPa and Ey = 112.35 GPa. Also, the Poisson’s ratios were

calculated asυx= 0.29 andυy= 0.30 by the linearﬁtting of the

transverse strain to axial strain curve up to 2% strain. Our work results are in good agreement with those in the literature, that is, 126.1 GPa andυ = 0.27.29In addition, the near-degeneracy of the elastic moduli along two orthogonal directions implies that the single-layer WS2 is a virtually elastic isotropic 2D

material because of the threefold rotational symmetry in this quasi-hexagonal lattice structure.34

As the applied strain increases, the relationship between stress and strain gradually becomes nonlinear. The maximum stress and its corresponding strain along the AC direction are higher than that along the ZZ direction. The obtained mechanical properties of stand-alone WS2 defect-free and

with S vacancy, 5−8−5, ZZ, AC-S, and AC-W defects are listed inTable 2. The corresponding results are also plotted inFigure 5. The monolayer WS2 with ZZ cracks is more likely to be

broken under the tensile stress along the AC direction, which is of 0.081 critical strain and 4.88 GPa ultimate stress. In the case of the stress along the ZZ direction, WS2with AC-S and AC-W

line defects tend to be more fragile, which are of 0.080 and
0.082 critical strain, respectively. In contrast, the critical strain
of WS_{2} with ZZ line defects signiﬁcantly increased to 0.199.
This is because the AC direction expansion of the original line
defect releases the localized stress, resulting in several spikes in
the stress−strain curve and a higher critical strain. The
simulation results show that the crack will seriously degrade
Figure 2.Schematic of the (a) top view and side view of six crack types in WS2: point defects of (a) 2S vacancies and (b) 5−8−5 defect; line
defects of (c) ZZ crack, (d) AC-S crack, and (e) AC-W crack. W atoms are shown in blue, whereas S atoms are shown in yellow.

Figure 3.Schematic of the WS2-basedﬂexible device.

Table 1. Material Properties of the Materials in WS2-Based

Flexible Devicea
item Au PET PI PDMS
dimension (mm) N/A
l× w × t:
50× 10 × 0.1/0.075/0.05/0.02
density (kg/m3_{)} _{19,300} _{2210} _{1420} _{1220}

Young’s module (GPa) 78.5 4.5 2.5 0.0018 Poisson’s ratio 0.42 0.37 0.34 0.48

the mechanical performance of the monolayer WS2with stress

perpendicular to its extension direction.

In AC-type defects, it can be seen that the ultimate stress of the AC-S crack is greater than that of the AC-W defect, which is mainly because of diﬀerent interatomic interactions between W−W and S−S atoms in WS2. As listed inTable S1, the cutoﬀ

distance of W−W pairwise interactions (rmax‑W−W= 4.3 Å) is

larger than that of S−S interactions (r_{max‑S−S}= 3.8 Å). Because
the distance between the four S atoms at the tip of AC-W is
larger than rmax‑S−S, they do not interact with each other. On

the contrary, the distance between the two W atoms (3.166 Å)
at the tip of the AC-S crack is less than r_{max‑W−W}; thus, they
interact with each other. As a result, a higher energy is needed
to deduce this extra interatomic interaction and deform the
crack tip neighborhood, which consequently leads to an
increase in the fracture strength. With regard to the 5−8−5
crack, the crack prefers to propagate along the ZZ edge, which
has a lower edge energy than the AC edge.35

Figure 4.Stress−strain curves of defect-free WS2, and WS2with 2S vacancies, 5−8−5, ZZ, AC-S, and AC-W defects for the tensile loading along (a) AC direction and (b) ZZ direction.

Table 2. Mechanical Properties of Defect-Free WS2and WS2with S Vacancy, 5−8−5, AC-S, AC-W, and ZZ Defects defect-free 2S defect 5−8−5 defect AC-S defect AC-W defect ZZ defect

AC E (GPa) 107.08 112.53 108.91 95.42 102.81 61.19 σ (GPa) 19.16 19.94 15.12 15.23 13.53 4.97 Ε 0.199 0.220 0.145 0.162 0.152 0.072 ZZ E (GPa) 105.92 111.93 106.98 106.49 110.90 101.28 σ (GPa) 14.44 13.50 11.63 8.22 7.16 9.88 Ε 0.142 0.149 0.111 0.076 0.075 0.132

Figure 5.Critical strain and elastic modulus of defect-free WS2, and WS2with 2S vacancies, 5−8−5, AC-S, AC-W, and ZZ defects for the tensile loading along (a) AC direction and (b) ZZ direction.

Figure 6.Stress distribution on atoms (a) at the strain ofε = 0.0, 0.190, 0.200 in the AC direction and (b) side view at ε = 0.190 for defect-free WS2.

To further study the stress distribution on each atom, the atomic stress map in MD simulations is plotted inFigures 6

and7for diﬀerent loading conditions. The transition from blue

to red shows an increase in the magnitude of the atomic stress during tensile deformation. Before the ﬁnal fracture, the proﬁles of atomic stress distribution are extracted to reveal the failure mechanism contributed by W and S atoms, respectively. As shown in Figure 6a, several microcracks in the S layers before the fracture appear, and the exposed W atoms exhibit a higher atomic stress than S atoms. From the side view in

Figure 6b, it can be veriﬁed that S atoms are colored in blue,

indicating a low atomic stress, whereas the major stress is concentrated in the W layer. In the loading along the ZZ direction shown inFigure 8, fewer cracks are observed in the S layers and from its proﬁle. It can be found that W atoms also exhibit a higher atomic stress. It is noticeable that the fracture is perpendicular to an AC loading direction but shows 30° in the case of a ZZ loading.

To ﬁgure out the inﬂuence of defects on the failure mechanism, the atomic stress distribution of each model before and after failure is shown in Figure 8 for the AC and ZZ directions. It can be seen that the ﬁnal fracture takes place Figure 7.Stress distribution on atoms (a) at the strain ofε = 0.0, 0.150, 0.160 in the ZZ direction and (b) side view at ε = 0.150 for defect-free WS2.

around the original defects. For the loading along the AC direction, similar to the defect-free model, a large number of cracks appear in S layers, and the stress concentrates in the W layer. The model with 2S defect shows the most cracks, resulting in the largest critical strain. In contrast, fewer cracks in S layers are found in the rest model, indicating a smaller critical strain. Especially in the model of ZZ defect, because of the large initial crack, the extension quickly happens, and WS2

breaks before many cracks formed in the S layers.

Furthermore, when the loading is in the ZZ direction, in the model of AC-S defect and AC-W defect, the initial defect becomes perpendicular to the loading force, resulting in a small critical strain, as 0.081 and 0.08, respectively. In contrast, the initial defect in the model of ZZ defect is parallel to the loading force. Therefore, the critical strain increases to 0.139, which is approximately twice the number with the AC direction loading, 0.078. It is also noticeable that theﬁnal failure takes place on the initial crack in the case of the two AC defect models. In the

model of ZZ defect, the failure position is at one end of the manually created ZZ defect. Besides, the models containing point defects present insensitivity to the loading direction. Similar to the defect-free model, the fracture exhibits 30°, and its critical strain is smaller than that of the model with the loading in the AC direction.

The atomic stress distribution near failure in defect-contained models show that point defects have less inﬂuence on the failure mechanism but lose the mechanical properties. As for models containing line defects, failure usually takes place on the initial cracks. Its ultimate stress and critical strain signiﬁcantly degrade when the loading direction is perpendic-ular to the crack direction.

3.2. Eﬀect of Defect Density on the Mechanical Performance of WS2. To comparatively analyze the eﬀects of

defect densities, a single defect was put in various simulation systems with diﬀerent dimensions to change the defect densities. The convergence of the mechanical properties with Figure 9.Stress−strain curve of uniaxial tension simulation in defect-free monolayer WS2at various dimensions: (a) loading along AC direction; (b) loading along ZZ direction.

Figure 10.Mechanical properties of the monolayer WS2with various defect densities. AC loading direction: (a) elastic modulus; (b) ultimate stress; (c) fracture strain; ZZ loading direction: (d) elastic modulus; (e) ultimate stress; (f) fracture strain.

system dimensions wasﬁrst veriﬁed with the defect-free model, as shown inFigure 9. It is found that the simulation system fell to equilibrium with a dimension of 75 Å, whereas the dimension over 100 Å presents a consistent result. As a result, a simulation system with 100 Å dimension contains suﬃcient atoms and therefore is proper to simulate tension under various conditions.

Then, the tension simulations of the three models along the AC and ZZ directions were conducted in diﬀerent-sized simulation boxes. The mechanical properties are plotted in

Figure 10, where each point presentsﬁve data, and the dashed line is theﬁtting line to the average values. It can be seen that the model with no defect and the one with 2S defect show similar mechanical properties and slight changes according to diﬀerent-sized simulation systems. This is because the missing S atom takes a negligible percentage to the whole system, such as 0.06, 0.04, and 0.03% in the simulation system, with dimensions of 100, 125, and 150 Å, respectively.

However, in the case of the AC-S defect model, the defect density is higher than the 2S defect model because of the line defect. The missing atoms in the line defect occupy 0.72, 0.62, and 0.54% in the three sized simulation systems. Therefore, in a larger simulation system, the defect density correspondingly decreases, resulting in a closer elastic modulus to the defect-free model as well as the 2S defect model. As for the ultimate stress and fracture strain, similar phenomena are observed along the AC direction such that the numbers in a 150 Å sized simulation system have neglect diﬀerences. In contrast, the obtained ultimate stress and fracture strain with ZZ direction loading present noticeable gaps compared to the obtained values in either the defect-free model or 2S defect model,

although a slight increase is still observed. It is due to the diﬀerent fracture mechanism that has been described in

Section 3.1.

Therefore, it can be concluded that a lower defect density indicates improved elastic modulus, close to a defect-free model. As for the ultimate stress and fracture strain, which are not the material’s intrinsic properties, defect density plays a less important role in the case of a line defect model because of the failure mechanism.

3.3. Eﬀect of Temperature on the Mechanical Performance of WS2. To study the eﬀect of temperature

on the mechanical behavior of the defect-free WS_{2}, MD
simulations of tensile tests are performed in the temperature
range of 200−600 K with an increment of 100 K. The
corresponding stress−strain curves are plotted inFigure 11for
AC and ZZ loading directions. It can be seen that under
loading along the AC direction, the ultimate stress decreases
with an increase in temperature. However, under a ZZ
direction loading, the ultimate stress changes slightly in the
temperature range of 200−400 K. To obtain a better
understanding of the eﬀects of temperature, the values of the
fracture strength, fracture strain, and Young’s modulus of the
monolayer WS2 as a function of temperature are plotted in

Figure 12, where each point represents the average of ﬁve points. As shown inFigure 11a, the loading direction has less inﬂuence on the elastic modulus, whereas the promotion caused by temperature is observed before 500 K. At 600 K, degradation from 115.39 to 104.62 and from 115.42 to 104.03 GPa is found in the AC and ZZ loading directions, respectively. As shown in Figure 12a, the loading direction has less inﬂuence on the elastic modulus, whereas the Figure 11.Stress−strain curve of uniaxial tension simulation in the defect-free monolayer WS2at various temperatures: (a) loading along the AC direction; (b) loading along the ZZ direction.

Figure 12.Mechanical properties of the monolayer WS2at diﬀerent temperatures. (a) Young’s modulus vs temperature; (b) fracture strain vs temperature; (c) ultimate stress vs temperature.

promotion caused by temperature is observed before 500 K. At 600 K, degradation from 115.39 to 104.62 and 115.42 to 104.03 GPa is found in the AC and ZZ loading directions, respectively. Besides, it is seen in Figure 12b that as the temperature increases from T = 200 K to T = 600 K, the fracture strain shows a slight increase in both loading directions, and the ductility along the AC loading direction is higher than the number along the ZZ direction at all tension temperatures. As for the ultimate stress, in contrast, inFigure 12c, a signiﬁcant decrease from 17.28 to 9.89 GPa is found along the AC direction. Similarly, with the temperature increasing to 600 K, this number also experiences a slighter decrease from 13.70 to 9.43 GPa along the AC direction.

The eﬀect of temperature on the strength of the monolayer
WS_{2} is analyzed as follows. First, according to the Arrhenius
equation, the lifetime τ has an exponential function with the
tensile stressσ and temperature T36,37

i
k
jjj y_{{}zzz
*T* *U*
*kT*
( , ) _{0}exp 0
*τ σ* =*τ* − γσ
(2)
whereτ0is the average period of vibrations of atoms in solids,

which is approximately 10−13 s, U_{0} is the fracture activation
energy, andγ is the product of the activation volume and the
coeﬃcient of local overstresses, and k is the Boltzmann’s
constant. The term U0− γσ means that the energy barrier for

brittle fracture can be lowered by increasing the tensile stress. Based on this function, Chung et al.35calculated the ultimate tensile stress σuts of graphene/silicene/graphene

heterostruc-tures as below:
i
k
jjjjj y_{{}zzzzz
*U* *kT* *kT*
*E*
ln
uts
0
0
*σ*
*γ* *γ* *γτ ε*
= −
̇ _{(3)}

where E is Young’s modulus and ε is the constant strain rate.
Because the variation of the logarithmic term with temperature
is negligible,σ_{uts} can be approximated as a linear function of
temperature. This formula can be used for WS2, as shown in

Figure 12; the linear plot suggests that the kinetic process leading to WS2 can be broken down into elementary events,

where the thermal vibration of the atoms leads to bond dissociation.

Therefore, it can be concluded that diﬀerent loading
directions exhibit diﬀerent sensitivities to temperature that
the ZZ direction is less inﬂuenced by temperature compared to
the AC direction. Thus, in the experimental design, loading
along the ZZ direction is recommended to be applied to WS_{2}.
Besides, the applied strain less than 0.14 and stress less than 10
GPa can be adopted as the boundary conditions in the
practical tension experiments.

3.4. Eﬀects of the Substrate on the Mechanical Performance of WS2-Based Devices. 3.4.1. Theoretical

Analysis. The performance of the strain sensor can be evaluated according to the GF, which is the ratio of relative change in electrical resistance (R) to the mechanical strainε (GF = (ΔR/R0)/ε). Thus, in our case, the GF of the WS2

strain sensor can be expressed as

*R* *R*

GF_{sensor} = Δ( _{total}/ _{total})/*ε*_{x}

where R_{total}= R_{WS2} + R_{Au}

*R*_{total} *R*_{WS2} *R*_{Au}

Δ = Δ + Δ

As the Au electrode oﬀers very little resistance, ΔR_{Au} ≈ 0,
RAu≈ 0

*R* *R*

GF_{sensor} = Δ( _{WS2}/ _{WS2})/*ε*_{x}

where the tensile strain εx is εx = F/(EΔS), F is the tensile

force, E is Young’s modulus of the substrate, and S is the cross-sectional area of the substrate.

It is obvious that GF_{sensor} depends on the electronic
properties of WS2 as well as the mechanical properties

(dimensions and Young’s modulus) of the substrate. There-fore, we analyzed the mechanical properties of the WS2 PET

strain sensor as an example. The FEA model and methods are described inSection 2.3. The left end isﬁxed, and the right end is applied with a tensile force F of 400 N in the x direction. As shown inFigure 13, the WS2PET device is with a length of 50

mm, width of 10 mm, and thickness of 75 μm. When F
increases to 400 N, the maximum equivalent elastic strain in
the center of the device can reach the critical strain of WS_{2}, 0.1.
The equivalent elastic strain of WS2ﬂexible devices is shown in

Figure 13, which reveals that the strain in the center of the sensor is aﬀected by the strain of the electrodes.

3.4.2. Benchmark Analysis. For benchmarking the FEA results, we fabricated a WS2strain sensor in a PET substrate.

As shown in Figure 14, a chemical vapor deposition-grown WS2 thin ﬁlm was transferred to the center of the PET

substrate. Then, Au electrodes were deposited to the top of the WS2 thin ﬁlm through the thermal evaporation process,

followed by a lift-oﬀ process. The thickness of the WS_{2} thin
ﬁlm is about 10 nm, as shown inFigure S1. Theﬂowchart of
the fabrication process is shown inFigure S2. The tensile test
was carried out through a homemadeﬁxture (seeFigure S3).
The real-time current change was reported by a source meter
(Keithley 2400). The measurement results show that the
current of the WS_{2} sensor increases when applying tensile
strain, which is consistent with the increased conductivity of
WS_{2}calculated from theﬁrst-principles analysis. The response
time is shorter than 10 s. It indicates that WS2has potential

applications in the strain sensor. However, the current change is so small, only 0.5 nA, which is associated with the slight deformation of the substrate under 397 N tensile force. The strain of PET is around 0.07, which is consistent with the strain value in the center of the FEA model. It means that our multiscale analysis can be used for benchmarking theﬂexible device.

3.4.3. Optimization of the Substrate. Because the
deformation of the substrate for the WS_{2}sensor is too small,
it is necessary to optimize the WS2structure to obtain a higher

GF. FEA was carried out to comparatively analyze the
relationship between the mechanical properties of the substrate
and tensile force (F). It is clear that the thicker the substrate,
the higher F is required to reach the critical strain of 0.1. We
should reduce the cross-sectional area of the substrate (S = w×
t, w: width, t: thickness) to decrease F. It can also be found that
F depends on Young’s module E of the substrate when S and ε_{x}
areﬁxed. In this case, it is better to choose one substrate with
low E to achieve a higher GF (Figure 15).

3.4.4. Eﬀects of Defects on the Electrical Performance of WS2. As the band structure can reveal the conductivity of a

material, the strains in AC (x) and ZZ (y) directions are
carried out for the monolayer WS_{2} by ﬁxing one lattice
constant and changing the other. As shown inFigure 16, the
electronic structures vary signiﬁcantly by the strain in both
defect-free and point defect-contained WS2. The band gap

energy (Eg) decreases linearly when the strain increases from 0

to 1% in AC and ZZ directions. In the case of the defect-free
model, the band gap decreases from 1.906 to 1.167 eV in the
AC direction and to 1.137 eV in the ZZ direction, whereas
after introducing two S vacancies, this number drops from
0.716 to 0.403 and 0.514 eV along the AC and ZZ directions,
respectively. According to the classical relation between E_{g}and
the electrical conductivity (σ) of materials,38

e( *E*g/2*kT*)

*σ ∝* − (4)

where k and T are Boltzmann’s constant and the temperature, respectively. Clearly, a lower Eg indicates a higher σ at the

given temperature. Thus, the conductivity of the WS2-based

device increases after applying tensile strain. This is consistent with the experimental results. Moreover, defects can result in a narrower band gap of WS2, which induces a higher current.

4. CONCLUSIONS

This work systematically analyzes the mechanical properties of WS2on a multiscale. The mechanical properties (i.e., Young’s

modulus and critical stress) of WS_{2}under diﬀerent strains are
analyzed by MD. The inﬂuence of diﬀerent defect types (i.e.,
point defects and line defects), defect density, and diﬀerent
ambient temperatures on the mechanical properties are
discussed. Toﬁgure out the inﬂuence of defects on the failure
mechanism, the atomic stress distribution of each model before
and after a fracture is studied. The results reveal that the
performance of line defect models is sensitive to the loading
Figure 14.Optical images of (a) WS2thinﬁlm under Au electrodes and (b) WS2strain sensor with the PET substrate. (c) Dynamic current change
under tensile strain. In the blue area, 397 N tensile force was applied to the sample.

Figure 15. Thickness−tensile force curve for diﬀerent types of substrates.

direction, regardless of the defect density. Temperature also plays an essential role in deciding its performance, as high temperature results in better ductility but strength. Also, a peak of elastic modulus is found at 500 K. Then, we discuss the eﬀects of diﬀerent substrates on the ﬂexible WS2 device

through FEA. Finally, a WS_{2}strain sensor based on PET was
fabricated for benchmarking the ﬁrst-principles analysis and
FEA results. The deformation of PET agrees with the FEA
results. As the strain increased, the current of the sensor
gradually increased, which was veriﬁed with the DFT results.
The band gap changes of WS2 under diﬀerent strains are

analyzed through theﬁrst-principles analysis. The results show
that as the strain increases, the band gap becomes smaller. The
conductivity consequently increases. This proves that this
multiscale simulation method can eﬃciently analyze the
mechanical properties of 2D materials with and without
defects. This method can provide a prediction of mechanical
performances of WS_{2} at atomic, molecular, and device levels,
which can be extended to analyze all other 2D materials.

## ■

ASSOCIATED CONTENT### *

sı Supporting InformationThe Supporting Information is available free of charge at

https://pubs.acs.org/doi/10.1021/acs.jpcc.0c09897.

Two-body (bond-bending) SW potential parameters for GULP; three-body (angle-bending) SW potential parameters for GULP; SW potential parameters for LAMMPs; and LAMMPS input ﬁles for tension simulations (PDF)

## ■

AUTHOR INFORMATIONCorresponding Author

Guoqi Zhang − Department of Microelectronics, Faculty of Electrical Engineering, Mathematics & Computer Science, Delft University of Technology, Delft 2628 CT, the Netherlands; Email:G.Q.Zhang@tudelft.nl

Authors

Hongyu Tang − Department of Microelectronics, Faculty of Electrical Engineering, Mathematics & Computer Science, Delft University of Technology, Delft 2628 CT, the Netherlands; orcid.org/0000-0002-2720-6709

Dong Hu − Department of Microelectronics, Faculty of Electrical Engineering, Mathematics & Computer Science, Delft University of Technology, Delft 2628 CT, the Netherlands; orcid.org/0000-0002-3739-5750

Zhen Cui − Department of Microelectronics, Faculty of Electrical Engineering, Mathematics & Computer Science, Delft University of Technology, Delft 2628 CT, the Netherlands

Huaiyu Ye − School of Microelectronics, Southern University of Science and Technology, Shenzhen 518055, China; Shenzhen Institute of Wide-bandgap Semiconductors, Shenzhen 518055, Guangdong, China; orcid.org/0000-0002-0385-4728

Complete contact information is available at:

https://pubs.acs.org/10.1021/acs.jpcc.0c09897

Author Contributions

∥_{H.T. and D.H. contributed equally to this work.}

Notes

The authors declare no competingﬁnancial interest.

## ■

ACKNOWLEDGMENTSThis work was supported by the National Key R&D Program of China (2018YFE0204600), the Key-Area Research and D e v e l o p m e n t P r o g r a m o f G u a n g D o n g P r o v i n c e (2019B010131001), and the Shenzhen Key Project for Basic Research (JCYJ20200109140822796).

## ■

REFERENCES(1) Novoselov, K. S.; Geim, A. K.; Morozov, S. V.; Jiang, D.; Zhang, Y.; Dubonos, S. V.; Grigorieva, I. V.; Firsov, A. A. Electric Field Effect in Atomically Thin Carbon Films. Science 2004, 306, 666.

(2) Iguiñiz, N.; Frisenda, R.; Bratschitsch, R.; Castellanos-Gomez, A. Revisiting the Buckling Metrology Method to Determine the Young’s Modulus of 2D Materials. Adv. Mater. 2019, 31, 1807150.

(3) Mehew, J. D.; Unal, S.; Torres Alonso, E.; Jones, G. F.; Fadhil Ramadhan, S.; Craciun, M. F.; Russo, S. Fast and Highly Sensitive Ionic-Polymer-Gated WS2 -Graphene Photodetectors. Adv. Mater. 2017, 29, 1700222.

(4) Wang, G.; Li, L.; Fan, W.; Wang, R.; Zhou, S.; Lü, J.-T.; Gan, L.; Zhai, T. Interlayer Coupling Induced Infrared Response in WS2 /MoS2 Heterostructures Enhanced by Surface Plasmon Resonance. Adv. Funct. Mater. 2018, 28, 1800339.

(5) Kang, K.; Godin, K.; Kim, Y. D.; Fu, S.; Cha, W.; Hone, J.; Yang, E.-H. Graphene-Assisted Antioxidation of Tungsten Disulfide Monolayers: Substrate and Electric-Field Effect. Adv. Mater. 2017, 29, 1603898.

(6) Tang, H.; et al. Ultra-High Sensitive No2 Gas Sensor Based on Tunable Polarity Transport in Cvd-Ws2/Igzo P-N Heterojunction. ACS Appl. Mater. Interfaces 2019, 11, 40850−40859.

(7) Tang, H.; Tan, C.; Yang, H.; Zheng, K.; Li, Y.; Ye, H.; Chen, X.; Fan, X.; Ren, T.; Zhang, G. Tunable Electronic and Optical Properties of the Ws2/Igzo Heterostructure Via an External Electric Field and Figure 16.Band gap of (a) defect-free WS2and (b) WS2with 2S vacancies under strain in AC and ZZ directions.

(11) Guo, H.; Lan, C.; Zhou, Z.; Sun, P.; Wei, D.; Li, C. Transparent, Flexible, and Stretchable Ws2 Based Humidity Sensors for Electronic Skin. Nanoscale 2017, 9, 6246−6253.

(12) Qi, H.-Y.; Mi, W.-T.; Zhao, H.-M.; Xue, T.; Yang, Y.; Ren, T.-L. A Large-Scale Spray Casting Deposition Method of Ws2 Films for High-Sensitive, Flexible and Transparent Sensor. Mater. Lett. 2017, 201, 161−164.

(13) Jeong, H. Y.; Jin, Y.; Yun, S. J.; Zhao, J.; Baik, J.; Keum, D. H.; Lee, H. S.; Lee, Y. H. Heterogeneous Defect Domains in Single-Crystalline Hexagonal Ws2. Adv. Mater. 2017, 29, 1605043.

(14) Zhao, X.; Dai, X.; Xia, C.; Wang, T. Structural Defects in Pristine and Mn-Doped Monolayer Ws2: A First-Principles Study. Superlattices Microstruct. 2015, 85, 339−347.

(15) Schuler, B.; et al. How Substitutional Point Defects in Two-Dimensional WS2 Induce Charge Localization, Spin-Orbit Splitting, and Strain. ACS Nano 2019, 13, 10520−10534.

(16) Wang, X.; Tabarraei, A.; Spearot, D. E. Fracture Mechanics of Monolayer Molybdenum Disulfide. Nanotechnology 2015, 26, 175703. (17) Talebi, H.; Silani, M.; Bordas, S. P. A.; Kerfriden, P.; Rabczuk, T. A Computational Library for Multiscale Modeling of Material Failure. Comput. Mech. 2014, 53, 1047−1071.

(18) Budarapu, P. R.; Gracie, R.; Yang, S.-W.; Zhuang, X.; Rabczuk, T. Efficient Coarse Graining in Multiscale Modeling of Fracture. Theor. Appl. Fract. Mech. 2014, 69, 126−143.

(19) Dadrasi, A.; Albooyeh, A. R.; Mashhadzadeh, A. H. Mechanical Properties of Silicon-Germanium Nanotubes: A Molecular Dynamics Study. Appl. Surf. Sci. 2019, 498, 143867.

(20) Ahangari, M. G.; Mashhadzadeh, A. H.; Fathalian, M.; Dadrasi, A.; Rostamiyan, Y.; Mallahi, A. Effect of Various Defects on Mechanical and Electronic Properties of Zinc-Oxide Graphene-Like Structure: A Dft Study. Vacuum 2019, 165, 26−34.

(21) Ghorbanzadeh Ahangari, M.; Salmankhani, A.; Imani, A. H.; Shahab, N.; Hamed Mashhadzadeh, A. Density Functional Theory Study on the Mechanical Properties and Interlayer Interactions of Multi-Layer Graphene: Carbonic, Silicon-Carbide and Silicene Graphene-Like Structures. Silicon 2019, 11, 1235−1246.

(22) Hamed Mashhadzadeh, A.; Fereidoon, A.; Ghorbanzadeh Ahangari, M. Combining Density Functional Theory-Finite Element Multi-Scale Method to Predict Mechanical Properties of Polypropy-lene/Graphene Nanocomposites: Experimental Study. Mater. Chem. Phys. 2017, 201, 214−223.

(23) Kumar, H.; Er, D.; Dong, L.; Li, J.; Shenoy, V. B. Elastic Deformations in 2d Van Der Waals Heterostructures and Their Impact on Optoelectronic Properties: Predictions from a Multiscale Computational Approach. Sci. Rep. 2015, 5, 10872.

(24) Luan, Q.; Yang, C.-L.; Wang, M.-S.; Ma, X.-G. First-Principles Study on the Electronic and Optical Properties of Ws2 and Mos2 Monolayers. Chin. J. Phys. 2017, 55, 1930−1937.

(25) Bui, V. Q.; Pham, T.-T.; Le, D. A.; Thi, C. M.; Le, H. M. A First-Principles Investigation of Various Gas (Co, H2o, No, and O2) Absorptions on a Ws2monolayer: Stability and Electronic Properties. J. Phys.: Condens. Matter 2015, 27, 305005.

(26) Delley, B. From Molecules to Solids with the Dmol3 Approach. J. Chem. Phys. 2000, 113, 7756−7764.

(27) Debbichi, L.; Eriksson, O.; Lebègue, S. Electronic Structure of Two-Dimensional Transition Metal Dichalcogenide Bilayers from Ab Initio Theory. Phys. Rev. B: Condens. Matter Mater. Phys. 2014, 89, 205311.

of Super High-Performance Thermoelectric Materials Based on Mos2/Ws2 Hybrid Nanoribbons. Sci. Rep. 2016, 6, 21639.

(32) Surblys, D.; Matsubara, H.; Kikugawa, G.; Ohara, T. Application of Atomic Stress to Compute Heat Flux Via Molecular Dynamics for Systems with Many-Body Interactions. Phys. Rev. E 2019, 99, 051301.

(33) Stukowski, A. Visualization and analysis of atomistic simulation data with OVITO-the Open Visualization Tool. Modell. Simul. Mater. Sci. Eng. 2009, 18, 015012.

(34) Born, M.; Huang, K.; Lax, M. Dynamical Theory of Crystal Lattices. Am. J. Phys. 1955, 23, 474.

(35) Chung, J.-Y.; Sorkin, V.; Pei, Q.-X.; Chiu, C.-H.; Zhang, Y.-W. Mechanical Properties and Failure Behaviour of Graphene/Silicene/ Graphene Heterostructures. J. Phys. D: Appl. Phys. 2017, 50, 345302. (36) Wei, C.; Cho, K.; Srivastava, D. Tensile Strength of Carbon Nanotubes under Realistic Temperature and Strain Rate. Phys. Rev. B: Condens. Matter Mater. Phys. 2003, 67, 115407.

(37) Slutsker, A. I.; Betekhtin, V. I.; Lee, J. C.; Yusupov, D.; Kadomtsev, A. G.; Amosova, O. V. Temperature Dependence of Rupture Strength of the Amorphous Alloy Ni82.1cr7.8si4.6fe3.1m-n0.3al0.1cu<0.1b2. Acta Mater. 2004, 52, 2733−2738.

(38) Roondhe, B.; Jha, P. K.“Haeckelite”, a New Low Dimensional Cousin of Boron Nitride for Biosensing with Ultra-Fast Recovery Time: A First Principles Investigation. J. Mater. Chem. B 2018, 6, 6796−6807.